OPEN Material properties and structure of natural graphite sheet Martin Cermak1*, Nicolas Perez1,2, Michael Collins3 & Majid Bahrami1*
Natural graphite sheet (NGS) is compressible, porous, electrically and thermally conductive material that shows a potential to be used in fuel cells, fow batteries, electronics cooling systems, supercapacitors, adsorption air conditioning, and heat exchangers. We report the results of an extensive material characterization study that focuses on thermal conductivity, thermal difusivity, electrical conductivity, coefcient of thermal expansion (CTE), compression strain, and emissivity. All the properties are density-dependent and highly anisotropic. Increasing the compression from 100 to 1080 kPa causes the through-plane thermal and electrical conductivities to increase by up to 116% and 263%, respectively. The properties are independent of the sheet thickness. Thermal and electrical contact resistance between stacked NGS is negligible at pressures 100 to 1080 kPa. In the in-plane direction, NGS follows the Wiedemann-Franz law with Lorenz number 6.6 × 10−6 W K− 2 . The in-plane CTE is low and negative (shrinkage with increasing temperature), while the through-plane CTE is high, increases with density, and reaches 33 × 10−6 K− 1 . Microscope images are used to study the structure and relate it to material properties. An easy-to-use graphical summary of the forming process and NGS properties are provided in Appendices A and B.
Natural graphite sheet (NGS) is a compressible, porous, electrically and thermally conductive material that has been used primarily to make sealing gaskets because of its ability to conform to rough surfaces, withstand high temperatures, and resist corrosive fuids. Presently, it is used—or considered to be used—in numerous applications, including bipolar plates in fuel cells and fow batteries for its electrical conductivity and chemi- cal stability 1,2,3, supercapacitors for its corrosion resistance 4,5, adsorption cooling systems for its high thermal difusivity 6, heat spreaders for its high in-plane thermal conductivity7,8, heat exchangers for its thermal con- ductivity and corrosion resistance9, and heat sinks for its thermal conductivity, low weight, and ease of forming into complex shapes 10,11. Multiple other names are used in the literature to refer to NGS, such as compressed exfoliated natural graphite (CENG), graphite foil, or fexible graphite. However, the term fexible graphite can be misleading because fexing thicker sheets results in a brittle fracture. NGS is manufactured from natural graphite fakes in a process that involves soaking the fakes in an interca- lation compound that penetrates between the graphite layers. During subsequent rapid heating, the vaporized compound forces the graphite layers apart, forming exfoliated natural graphite (ENG) particles also known as − worms13. NGS at densities 0.5 to 1.73 g cm 3 is formed by compressing ENG particles at pressures ranging from 1 to 31 MPa6,14,15. In this study, we measure an extensive set of material properties and relate them to the structure observed by an SEM microscope. Te sheet density is the primary parameter with the strongest infuence on the properties. We found the through-plane thermal and electrical conductivity to increase with through–plane compression, and observed that the increase is density-dependent. Te thickness of the sheet did not afect the measured properties. − − − − − − Te through–plane conductivities are low ( 2 Wm 1K 1 to 6 Wm 1K 1 and 3 Scm 1 to 25 Scm 1 ) while the − − − − − − in-plane ones are high (100 Wm 1K 1 to 350 Wm 1K 1 and 500 Scm 1 to 1700 Scm 1 ). In the in–plane direc- tion, both thermal and electrical conductivities increase linearly with density. At low densities, our results agree with the previous studies, but at high densities we observed values 20 % to 25 % lower than those reported in the literature17,18,20. In the through–plane direction, the conductivities decrease with density. Te data from previous studies6,19,20,21,22 show high scatter and incomplete coverage of the density spectrum, which prevented us from forming a clear comparison with our results. Te thermal and electrical contact resistance between stacked sheets
1Laboratory for Alternative Energy Conversion, School of Mechatronic Systems Engineering, Faculty of Applied Science, Simon Fraser University, 250‑13450 102 Avenue, Surrey, BC V3T 0A3, Canada. 2The Institut National des Sciences Appliquées de Lyon, 20 Avenue Albert Einstein, 69621 Villeurbanne Cedex, France. 3Solar Thermal Research Laboratory, Department of Mechanical and Mechatronics Engineering, University of Waterloo, 200 University Avenue West, Waterloo, ON N2L 3G1, Canada. *email: [email protected]; [email protected]
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 1 Vol.:(0123456789) www.nature.com/scientificreports/
of NGS is negligible at pressures higher than 100 kPa. We found the emissivity at wavelengths from 2 to 26 µm to decrease with density in the range 0.39 to 0.52. ◦ When heated from room temperature to 100 C , NGS shows a dimensional stability superior to conven- tional materials such as aluminum or copper, however, the expansion in the through-plane direction is high and strongly dependent on the density. Our measurements show a very low and negative coefcient of thermal − − − − expansion (CTE) in the in–plane direction (− 0.6 × 10 6K 1 to −1.4 × 10 6K 1 ) while in the through-plane − − − − direction it is positive and ranges from 10 × 10 6 K 1 to 33 × 10 6 K 1 . Coupling the results with our study of the compression behaviour (outlined here and detailed elswhere 15) allows for a quantitative analysis of thermo- mechanical stresses in devices such as fuel cells. Te structure of NGS is composed of tens-of-nanometers thin, highly anisotropic graphitic features whose orientation, spacing, and contact quality dictate the overall macroscopic properties of NGS. Compressing NGS causes reversible and irreversible structural changes that refect in the overall properties. Te irreversible changes happen during the forming process, and the reversible ones during the low-pressure loading of a fnished sheet 15. In summary, the goal of the present study is to compile a comprehensive resource describing the NGS prop- erties and their relationship with the material structure. While the authors believe that this is the most com- prehensive resource to date, we clearly state the need for further research. Te most pressing issue is the lack of understanding of how the parameters of exfoliation methods and raw graphite fakes afect the structure and material properties of NGS. Results We frst describe the structure of NGS, and then address each of the measured material properties. Te forming process is not covered in this publication, however, a brief summary is provided in Appendix A. Te reader is referred to other publication 15 for details. Alongside the detailed description of the measurements and results further in this section, a simplifed graphical summary of the measured material properties with explicit formulas of best fts is provided in Appendix B.
Structure. Te structure of NGS is a result of compaction of ENG particles that are composed of highly crys- talline cell walls13 as can be seen in Appendix A. Te cell walls are 15 nm to 60 nm thick14,37 and their dimensions in the a and b crystal directions are equal to or less than the size of raw fakes38. Upon compression, the cell walls within a single ENG particle deform into a platelet shape32 but the particles remain cohesive14. Te cross-section structure at macro scale (hundreds of micrometers, Fig. 1a) changes signifcantly with the sheet density. At low densities, it is heterogenous with large slit shape pores, and becomes homogeneous at higher densities. Stitched images in Supplementary Figure S1 do not show the through-plane density variation predicted by Bonnissel et al.19. At the scale of tens of micrometers (Fig. 1b), the microscope images show layers of fattened ENG particles whose preferred orientation increases with increasing density. Previous X-ray dif- fraction stuides14,22,30,31 state that the mean angle of graphite basal planes with respect to the sheet plane varies ◦ ◦ − from 9 to 20 and that its change with sheet density is low at densities higher than 0.5 g cm 3 . Assuming that the the linear features in Fig. 1b correlate with the graphite basal planes, the observed angles are qualitatively consistent with the previous work. Te highest-magnifcation images at a micrometer scale shown in Fig. 1c reveal thin features whose thickness and spacing decrease with increasing density. Te decrease of thickness with increasing density suggests that the features are not crystalline because graphite crystals are not expected to undergo permanent thickness reduction under compression at pressures relevant to NGS. Te achieved level of magnifcation prevents forming defnitive conclusions, however, we interpret the thin features as clusters of cell walls whose porosity allows for their thickness to be reduced by the pressure during the forming process. Te images of sheet faces shown in Fig. 1d,e indicate that the surface structure changes from rough to smooth with increasing density. Te boundaries of the ENG particles are visible in the low magnifcation image of the − − 0.55 g cm 3 and 1.05 g cm 3 sheets. At higher densities, the surface appears uniform at low magnifcations, and signs of overlapping cell walls are apparent in the high magnifcation images. For relating the structure of NGS to its material properties, it should be noted that crystalline graphite is highly anisotropic. Te orientation of crystalline cell walls dictate the anisotropy of NGS. At high NGS densities, the cell walls are aligned parallel to the sheet plane, which leads to the properties closer to those of a graphite crystal. However, due to porosity, imperfect contact between the cell walls, crystal defects, and other imperfec- tions, the properties never reach those of a graphite crystal.
Material properties. Te measured in-plane thermal and electrical conductivities ( kin and σin ) increase linearly with density as is shown in Fig. 2a,c. In the through-plane direction, the thermal and electrical conduc- tivites ( kth and σth ) decrease with density as can be seen in Fig. 2b,d. Both kth and σth increase with through-plane compression pressure. For kth , the increase is not signifcant at low densities, but becomes progressively higher with increasing density. For kth , the increase is approximately constant over the entire measured density range. Te experimental methods employed in this study are not suitable for measuring kth and σth at pressures below 100 kPa due to the high and unpredictably variable contact resistance between sensors and samples. Attempts of low-pressure measurements indicated a steep decrease in kth and σth , but future measurements using novel methods are necessary to confrm or reject the observed trend. Measurement of kin at varying pressures did not reveal a pressure dependence, and the in-plane electrical conductivity σin was measured in uncompressed state only.
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 2 Vol:.(1234567890) www.nature.com/scientificreports/
Figure 1. Microscope images of NGS cross-section (a–c) and face (d, e). Te high-magnifcation cross-section images c) have been rotated to demonstrate the change of thickness and spacing of cell walls and they do not represent the orientation angle accurately. High-resolution images are available in the supplementary dataset 36.
Within the measured range of densities, pressures, and thicknesses, the thermal and electrical conductivities do not vary signifcantly with the sheet thickness, which can be supported by the overlap of the triangle and cir- cular symbols in Fig. 2. Te diferent sample thickness was achieved by using NGS at three surface densities (d s ) − of 70, 140 and 210 mg cm 2 . Since stacks of NGS were measured in the through-plane direction, the insignifcant variation with sheet thickness also suggests that the electric and thermal contact resistance at the sheet-to-sheet interfaces is negligible within the measured pressure range 100 kPa to 1080 kPa. − Te low density of NGS results in high thermal difusivity ranging from 230 to 270 mm2s 1 in the in-plane 2 −1 direction ( αin ) and from 1.5 to 12 mm s in the through-plane direction ( αth ). Te plots of thermal difusivity versus density are given in Appendix B. Te magnitude of thermal and electrical conductivity is dictated by the conductivity and orientation of the cell walls and the contact resistance between them. In the in-plane direction, the increase of kin and σin with density arises from the decrease of cell wall misalignment and the decreased contact resistance due to improved contact quality or formation of new contact points. In the through–plane direction, the observed decrease of kth and σth is contrary to the structure features seen in Fig. 1a,c. Closing of the slit-shaped pores and the decrease of the cell wall spacing with increasing density is expected to increase the through-plane conductivities. However, since the measured trend is opposite, the decrease in cell wall misalignment must be the dominating factor. Besides the density and through-plane compression pressure, the material properties of NGS have been 17,22 44 14,45 shown to be afected by the apparent density of ENG particles dENG , fake size , impurity content , crystal
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 3 Vol.:(0123456789) www.nature.com/scientificreports/
Figure 2. Te (a) in-plane thermal conductivity kin , (b) through-plane thermal conductivity kth , (c) in-plane electrical conductivity σin , and (d) through-plane electrical conductivity σth as a function of NGS density.
defects46, rolling direction14, or heat treatment14,47. A comparison of the present thermal and electrical con- ductivities with the literature values 6,17,18,19,20,21,22,39 is given in Supplementary Figures S2 and S3, but since the relevant parameters are varying or have not been reported, it is not possible to reliably explain the reasons for observed diferences. Moreover, diferent measurement methods were used across the literature sources, which further broadens the list of possible sources of the discrepancies. Extensive future work is required to evaluate the sensitivity of NGS properties to the parameters listed above. Te detailed compression behavior of kth and σth together with the through-plane stress-strain compression curves for three selected densities is shown in Fig. 3a–c. Te change of kth with pressure is qualitatively pro- −3 portional to the through-plane compression strain Sth . Both kth and Sth of the 0.55 g cm sheet show a linear increase with pressure. At higher densities, kth and Sth become progressively nonlinear with a higher rate of change at low pressures. Te through-plane electrical conductivity σth does not show the same proportionality to Sth as kth . Te relative increase of kth and σth at 1080 kPa with respect to the values at 100 kPa was plotted in Fig. 3d. Te pressure sensitivity increases with increasing density, and σth is more sensitive to pressure than kth . Te increase of kth and σth with pressure is likely caused by the elastic deformation of cell walls and the improved contact quality between them, as is shown in Fig. 3e. Contrary to the forming process, no signifcant change in the misalignment of cell walls is expected. To verify the claim that NGS follows the Wiedemann–Franz law21, Lorenz number was calculated and plotted − − in Fig. 4 where it is seen to remain constant at 6.6 × 10 6 W K 2 in the in-plane direction, but increase in the
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 4 Vol:.(1234567890) www.nature.com/scientificreports/
Figure 3. Te pressure dependence of (a) through-plane electrical conductivity and (b) through-plane thermal conductivity with (c) through-plane compression strain. Te relative increase of the through-plane thermal − and electrical conductivities at 1080 kPa relative to 100 kPa is shown in (d). Only the 140mg cm 2 samples are shown to improve plot clarity. A schematic of the change of NGS structure with through-plane compression is shown in (e).
through-plane direction. Te Wiedemann–Franz law is therefore concluded to be valid in the in-plane direction, but not in the through-plane direction. Te in–plane CTE of NGS (CTE in ) shown in Fig. 5a is low, negative, and its magnitude increases with density. −6 −1 CTE in the through-plane direction (CTE th ) is large, positive, and increases with density up to 33 × 10 K as is shown in Fig. 5b. Te anisotropy and density dependence arises from the NGS structure, which was illustrated −6 −1 in Fig. 5c. At room temperature, the CTE of cell walls is −1.8 × 10 K in the ab crystal directions (CTE ab,gr ) −6 −1 41,42,43 and 26 × 10 K in the c direction (CTE c,gr) . Te deformation of a single cell wall with increasing temperature was outlined in Fig. 5d where the arrows symbolize the direction and magnitude of the dimension change. Te CTE of NGS is dictated by the orientation and interaction of all cell walls. At high densities, CTEin −3 approaches CTEab,gr as expected based on the highly-oriented structure. At densities above 1.2 g cm , CTEth appears to be higher than CTEc,gr , which is contrary to the expectations. However, the measurement uncertainty
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 5 Vol.:(0123456789) www.nature.com/scientificreports/
Figure 4. Lorenz number of NGS in the in-plane and through-plane directions as a function of density. Only − the results for 140 mg cm 2 samples are shown to improve plot clarity.
Figure 5. Results of CTE measurements in (a) in-plane and (b) through-plane directions. Te relevant graphite 41,42,43 crystal values CTEab,gr and CTEc,gr are demarcated by the dotted lines. In (c) a schematic structure of NGS is shown, and (d) illustrates the deformation of a single cell wall with increasing temperature.
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 6 Vol:.(1234567890) www.nature.com/scientificreports/
Figure 6. (a) Te total emissivity of NGS versus the free-standing density, (b) an illustration of the change of the in-plane electrical conductivity σin and surface structure with NGS density.
prevents a defnitive conclusion. It is likely that the expansion of air in the pores or the residual intercalation agent between graphite layers can cause an increase in CTEth beyond CTEc,gr. Te total emissivity at faces of NGS for wavelengths 2 µm to 26 µm decreases with increasing density, from − − 0.52 at 0.55g cm 3 to 0.39 at 1.7 g cm 3 as shown in Fig. 6a. Te emissivity of graphitic materials has been pre- 49 viously related to the in-plane electrical conductivity σin and surface roughness . As shown in the simplifed illustration in Fig. 6b, σin increases with increasing density, while the surface structure changes from rough to smooth. Both of the factors contribute to the decrease in emissivity, the former via the Hagen–Rubens relation49, and the latter via an increased surface area and the small pores that act as radiation black bodies. Experimental methods In-plane and through-plane thermal conductivities were measured using the transient plane source method (Hot Disk TPS 2500S) in the slab and one-dimensional modes, respectively. Electrical conductivity was measured using a four probe method with the Raytech Micro Junior 2 micro ohm meter. Te compression behavior was measured in a mechanical tester with circular compression platens 50 mm in diameter and 3 kN load cell (Bose Electroforce 3300 Series II). CTE was measured using a thermomechanical analyzer (TA Instruments TMA Q400). Emissivity was determined from refectivity measurements, which were performed in accordance with the Method C of ASTM E408-13 using an infrared refectometer (Surface Optics Corporation 400T). All measure- ◦ ◦ ments were performed at room temperature except for CTE, which was determined in the range 30 C to 100 C . − Te samples were prepared by calendering a low-density 0.2 g cm 3 NGS into the desired density and thickness. NGS was supplied by Nano Carbon Technology CO. and its properties were fxed carbon content 99.27 %, dENG −3 4 mg cm , fake size composition 81 % larger than 300 µm (50 mesh, before exfoliation), intercalation agent H 2 ◦ SO4+H2O2+KMnO4 , exfoliation temperature 950 C , and exfoliation time 5 min. A number of samples was tested to capture the variability of the properties. For example, for the through-plane thermal conductivity, 20 samples were prepared for each of the measured densities, resulting in the total of 240 samples. A random combination of 20 samples was measured at least three times at each of the compression pressures, which resulted in the total of 222 measurements. Te density of the samples was determined by measuring the dimensions and weight using an OHAUS AX124 scale and a Darson Instruments 0-1” analog micrometer. Te samples for cross-section SEM images were prepared by impregnating NGS in epoxy resin, polishing, and removing the smeared fakes by plasma etching. FEI Nova NanoSEM microscope was used for imaging. Te compression behavior measurements were reported elsewhere 15. Details about the measurement methods, sample preparation, and uncertainty analysis were addressed at length in the supplementary document. Te raw data, data processing scripts, microscope images in high resolution, and results in a tabular form are available in the supplementary dataset 36.
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 7 Vol.:(0123456789) www.nature.com/scientificreports/
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 8 Vol:.(1234567890) www.nature.com/scientificreports/
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 9 Vol.:(0123456789) www.nature.com/scientificreports/
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 10 Vol:.(1234567890) www.nature.com/scientificreports/
Received: 29 April 2020; Accepted: 13 October 2020
References 1. Qian, P. et al. A novel electrode-bipolar plate assembly for vanadium redox fow battery applications. Journal of Power Sources 175, 613 – 620 (2008). http://www.sciencedirect.com/science/article/pii/S0378775307017806. 2. Lourenssen, K., Williams, J., Ahmadpour, F., Clemmer, R. & Tasnim, S. Vanadium redox fow batteries: A comprehensive review. Journal of Energy Storage 25, 100844 (2019). http://www.sciencedirect.com/science/article/pii/S2352152X19302798. 3. Kopasz, J. P., Benjamin, T. G. & Schenck, D. bipolar plate workshop summary report. Tech. Rep., Argonne National Lab.(ANL), Argonne, IL (United States) (2017). 4. Blomquist, N. et al. Metal-free supercapacitor with aqueous electrolyte and low-cost carbon materials. Scientifc reports 7, 39836 (2017). 5. Blomquist, N., Koppolu, R., Dahlström, C., Toivakka, M. & Olin, H. Infuence of substrate in roll-to-roll coated nanographite electrodes for metal-free supercapacitors. Scientifc Reports 10, 1–9 (2020). 6. Wang, L., Metcalf, S., Critoph, R., Torpe, R. & Tamainot-Telto, Z. Termal conductivity and permeability of consolidated expanded natural graphite treated with sulphuric acid. Carbon 49, 4812 – 4819 (2011). http://www.sciencedirect.com/science/article/pii/ S0008622311005422. 7. Chung, D. & Takizawa, Y. Performance of isotropic and anisotropic heat spreaders. Journal of Electronic Materials 41, 2580–2587 (2012). https://doi.org/10.1007/s11664-012-2177-4. 8. Termal Performance of Natural Graphite Heat Spreaders, vol. Advances in Electronic Packaging, Parts A, B, and C of International Electronic Packaging Technical Conference and Exhibition. 10.1115/IPACK2005-73073. https://asmed igita lcoll ectio n.asme.org/Inter PACK/proceedings-pdf/InterPACK2005/42002/79/4531386/79_1.pdf. 9. Jamzad, P., Kenna, J. & Bahrami, M. Development of novel plate heat exchanger using natural graphite sheet. International Journal of Heat and Mass Transfer 131, 1205 – 1210 (2019). http://www.sciencedirect.com/science/article/pii/S0017931018337098. 10. Norley, J., Tzeng, J. J. ., Getz, G., Klug, J. & Fedor, B. Te development of a natural graphite heat-spreader. In Seventeenth Annual IEEE Semiconductor Termal Measurement and Management Symposium (Cat. No.01CH37189), 107–110 (2001). 11. Cermak, M., Faure, X., Saket, M. A., Bahrami, M. & Ordonez, M. Natural graphite sheet heat sinks with embedded heat pipes. IEEE Access 8, 80827–80835 (2020). 12. Kaburagi, Y., Aoki, H. & Yoshida, A. Termal and electrical conductivity and magnetoresistance of graphite flms prepared from aromatic polyimide flms. Tanso 5–9, (2012). 13. Chung, D. D. L. A review of exfoliated graphite. Journal of Materials Science 51, 554–568 (2016). https://doi.org/10.1007/s1085 3-015-9284-6. 14. Dowell, M. & Howard, R. Tensile and compressive properties of fexible graphite foils. Carbon 24, 311 – 323 (1986). http://www. sciencedirect.com/science/article/pii/0008622386902320. 15. Cermak, M. & Bahrami, M. Compression behavior of natural graphite sheet. SN Applied Sciences 2, 357 (2020). 16. Chung, D. D. L. Exfoliation of graphite. Journal of Materials Science 22, 4190–4198. https://doi.org/10.1007/BF01132008 (1987). 17. Wei, X. H., Liu, L., Zhang, J. X., Shi, J. L. & Guo, Q. G. Mechanical, electrical, thermal performances and structure characteristics of fexible graphite sheets. Journal of Materials Science 45, 2449–2455. https://doi.org/10.1007/s10853-010-4216-y (2010). 18. Liu, R. et al. Anisotropic high thermal conductivity of fexible graphite sheets used for advanced thermal management materials. In 2013 International Conference on Materials for Renewable Energy and Environment, vol. 1, 107–111 (2013). 19. Bonnissel, M., Luo, L. & Tondeur, D. Compacted exfoliated natural graphite as heat conduction medium. Carbon 39, 2151 – 2161 (2001). http://www.sciencedirect.com/science/article/pii/S000862230100032X. 20. Luo, X. & Chung, D. Electromagnetic interference shielding reaching 130 db using fexible graphite. MRS Proceedings 445, 235 (1996). 21. Chen, P.-H. & Chung, D. Termal and electrical conduction in the compaction direction of exfoliated graphite and their relation to the structure. Carbon 77, 538 – 550 (2014). http://www.sciencedirect.com/science/article/pii/S0008622314005132. 22. Afanasov, I. M. et al. Termal conductivity and mechanical properties of expanded graphite. Inorganic Materials 45, 486–490. https://doi.org/10.1134/S0020168509050057 (2009). 23. Gu, J. L., Leng, Y., Kang, E. & Shen, W. C. Microstructure efect on mechanical properties of fexible graphite sheet. Engineering Fracture Mechanics (1985). http://citeseerx.ist.psu.edu/viewdoc/summary?doi=10.1.1.617.1336. 24. Gu, J. et al. Fracture mechanism of fexible graphite sheets. Carbon 40, 2169 – 2176 (2002). http://www.sciencedirect.com/scien ce/article/pii/S0008622302000751. 25. Ionov, S. G., Avdeev, V. V., Kuvshinnikov, S. V. & Pavlova, E. P. Physical and chemical properties of fexible graphite foils. Molecular Crystals and Liquid Crystals Science and Technology. Section A. Molecular Crystals and Liquid Crystals 340, 349–354 (2000). https ://doi.org/10.1080/10587250008025491. 26. Luo, X. & Chung, D. Flexible graphite under repeated compression studied by electrical resistance measurements. Carbon 39, 985 – 990 (2001). http://www.sciencedirect.com/science/article/pii/S000862230000213X. 27. Chen, P.-H. & Chung, D. Viscoelastic behavior of the cell wall of exfoliated graphite. Carbon 61, 305 – 312 (2013). http://www. sciencedirect.com/science/article/pii/S0008622313004223. 28. Luo, X., Chugh, R., Biller, B. C., Hoi, Y. M. & Chung, D. D. L. Electronic applications of fexible graphite. Journal of Electronic Materials 31, 535–544. https://doi.org/10.1007/s11664-002-0111-x (2002). 29. Chung, D. D. L. Flexible graphite for gasketing, adsorption, electromagnetic interference shielding, vibration damping, electrochem- ical applications, and stress sensing. Journal of Materials Engineering and Performance 9, 161–163. https://doi.org/10.1361/10599 4900770346105 (2000). 30. Gu, J. L., Cao, W. Q., Cao, N. Z. & Shen, W. C. Efect of mictrostructure on compressive properties of fexible graphite sheet. In Te European Carbon Conference “Carbon 96”, 346–347 (1996). 31. Celzard, A., Schneider, S. & Marêché, J. Densifcation of expanded graphite. Carbon 40, 2185 – 2191 (2002). http://www.sciencedir ect.com/science/article/pii/S0008622302000775. 32. Toda, H. et al. Compression and recovery micro-mechanisms in fexible graphite. Carbon 59, 184 – 191 (2013). http://www.scien cedirect.com/science/article/pii/S0008622313002273. 33. Spencer, H. Empirical heat capacity equations of gases and graphite. Ind. and Eng. Chem. 40, (1948). 34. Cermak, M., Collins, M. & Bahrami, M. Emissivity of natural graphite sheet. International Journal of Heat and Mass Transfer (2020). Under review. 35. Cermak, M. Natural graphite sheet heat sinks for power electronics. Ph.D. thesis, Simon Fraser University (2020). 36. Cermak, M., Perez, N. & Bahrami, M. Material properties and structure of natural graphite sheet - dataset. https://doi.org/10.20383 /101.0216 (2020). 37. Celzard, A., Marêché, J. & Furdin, G. Surface area of compressed expanded graphite. Carbon 40, 2713 – 2718 (2002). http://www. sciencedirect.com/science/article/pii/S0008622302001835. 38. Celzard, A., Marêché, J. F. & Furdin, G. Modelling of exfoliated graphite. Progress in Materials Science 50, 93–179 (2005).
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 11 Vol.:(0123456789) www.nature.com/scientificreports/
39. Celzard, A., Mareche, J., Furdin, G. & Puricelli, S. Electrical conductivity of anisotropic expanded graphite-based monoliths. Journal of Physics D: Applied Physics 33, 3094 (2000). 40. Inagaki, M., Kaburagi, Y. & Hishiyama, Y. Termal management material: Graphite. Advanced Engineering Materials 16, 494–506 (2014). https://onlinelibrary.wiley.com/doi/abs/10.1002/adem.201300418. 41. Pierson, H. O. 3 - graphite structure and properties. In Pierson, H. O. (ed.) Handbook of Carbon, Graphite, Diamonds and Fullerenes, 43 – 69 (William Andrew Publishing, Oxford, 1993). http://www.sciencedirect.com/science/article/pii/B9780815513391500086. 42. Kelly, B. T. B. T. Physics of graphite / B.T. Kelly. (Applied Science, London ; Englewood, N.J., 1981). 43. Tsang, D., Marsden, B., Fok, S. & Hall, G. Graphite thermal expansion relationship for diferent temperature ranges. Carbon 43, 2902 – 2906 (2005). http://www.sciencedirect.com/science/article/pii/S0008622305003374. 44. Leng, Y., Gu, J., Cao, W. & Zhang, T.-Y. Infuences of density and fake size on the mechanical properties of fexible graphite. Carbon 36, 875 – 881 (1998). http://www.sciencedirect.com/science/article/pii/S0008622397001966. 45. Smalc, M., Norley, J., Reynolds, R. A., Pachuta, R. & Krassowski, D. W. Advanced Termal Interface Materials Using Natural Graphite. In 2003 International Electronic Packaging Technical Conference and Exhibition, Volume 2, 253–261 (2003). http://proce edings.asmedigitalcollection.asme.org/proceeding.aspx?doi=10.1115/IPACK2003-35113. 46. Hooker, C. N., Ubbelohde, A. R. J. P. & Young, D. A. Termal conductance of graphite in relation to its defect structure. Proceedings of the Royal Society of London. Series A. Mathematical and Physical Sciences 276, 83–95 (1963). 10.1098/rspa.1963.0194. 47. Kitaoka, S., Wada, M., Nagai, T., Osa, N. & Konno, T. Increasing the thermal difusivity of fexible graphite sheets by superheated steam treatment. Journal of Materials Science 46, 1132–1135. https://doi.org/10.1007/s10853-010-4991-5 (2011). 48. Uher, C., Hockey, R. L. & Ben-Jacob, E. Pressure dependence of the c-axis resistivity of graphite. Phys. Rev. B 35, 4483–4488. https ://doi.org/10.1103/PhysRevB.35.4483 (1987). 49. Autio, G. & Scala, E. Te normal spectral emissivity of isotropic and anisotropic materials. Carbon 4, 13 – 28 (1966). http://www. sciencedirect.com/science/article/pii/0008622366900054. Acknowledgements Te authors are thankful for the fnancial support provided by the Natural Sciences and Engineering Research Council of Canada under the College-University Idea to Innovation Grant number 470927-14. Tis work made use of the 4D LABS shared facilities supported by the Canada Foundation for Innovation (CFI), British Columbia Knowledge Development Fund (BCKDF), Western Economic Diversifcation Canada (WD) and Simon Fraser University (SFU). John Kenna and Shoji Kanamori of Terrella Energy Systems kindly provided their expertise in NGS forming. Xin Zhang of 4D labs provided the training and helpful feedback during SEM imaging. Wendell Huttema and Claire McCague proofread the manuscript and ofered valuable comments. Author contributions M.Ce. identifed the research needs, reviewed literature, planned and troubleshooted the experimental methods, prepared samples, collected data, analyzed results, prepared fgures, and wrote the manuscript. N.P. planned and troubleshooted the experimental methods, prepared samples, collected data, and analyzed the results. M.Co. planned and performed the emissivity measurements. M.B. initiated and supervised the project and secured funding. All authors have reviewed the manuscript.
Competing interests Te authors declare no competing interests. Additional information Supplementary information is available for this paper at https://doi.org/10.1038/s41598-020-75393-y. Correspondence and requests for materials should be addressed to M.C. or M.B. Reprints and permissions information is available at www.nature.com/reprints. Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afliations. Open Access Tis article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. Te images or other third party material in this article are included in the article’s Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http://creativecommons.org/licenses/by/4.0/.
© Te Author(s) 2020
Scientifc Reports | (2020) 10:18672 | https://doi.org/10.1038/s41598-020-75393-y 12 Vol:.(1234567890)